| ||Format||Pages||Price|| |
|5||$48.00||  ADD TO CART|
|Hardcopy (shipping and handling)||5||$48.00||  ADD TO CART|
Significance and Use
5.1 These test methods provide a quantitative measure of the pressure-sensitive tack property of an adhesive.
FIG. 1 Loop Tack Test Fixture 1
FIG. 2 Loop Tack Test Fixture 2
FIG. 3 Loop Tack Sample During Test
5.2 These test methods are designed to measure the tack property of the adhesive mass. The tack of a given adhesive varies depending on the backing (generally, stiffer backings lead to higher values).
5.3 Theses test methods are suitable for quality control and research purposes.
5.4 Test Method A (using Tensile Tester) makes use of a specimen strip 7 in. (175 mm) in length. Both the FINAT FTM 9 “Quick Stick” Tack Measurement Test and the TLMI L-IB2 Tensile Tester Loop Tack Test also use a specimen strip of that length.
5.5 Test Method B (using Loop Tack Tester) makes use of a specimen strip five in. (125 mm) in length. That is the only length specimen strip that fits properly in the loop tack tester.
5.6 If the adhesive is not already otherwise coated, these test methods incorporate the use of a clear 2 mil (0.05 mm) polyester (PET) film backing for specimen preparation. Use of other backing materials changes performance of the specimen to be tested.
1.1 These test methods cover the determination of properties of a pressure-sensitive adhesive. These test methods are applicable to those adhesives that form a bond of measurable strength rapidly upon contact with another surface. Tack force may be measured as the force required to separate the adhesive from the adherend at the interface shortly after they have been brought into contact under a load equal only to the weight of the pressure-sensitive article (for example, tape, label, sticker, etc.) on a 1 in.2 contact area.
1.2 The following test methods are included:
1.2.1 Test Method A (using Tensile Tester), and
1.2.2 Test Method B (using Loop Tack Tester).
1.3 The values stated in inch-pound units are to be regarded as the standard because the industry standard width for pressure-sensitive tape is 1 inch. The values given in parentheses are mathematical conversions to SI units that are provided for information only and are not considered standard.
1.4 This standard does not purport to address all of the safety concerns, if any, associated with its use. It is the responsibility of the user of this standard to establish appropriate safety, health, and environmental practices and determine the applicability of regulatory limitations prior to use.
1.5 This international standard was developed in accordance with internationally recognized principles on standardization established in the Decision on Principles for the Development of International Standards, Guides and Recommendations issued by the World Trade Organization Technical Barriers to Trade (TBT) Committee.
2. Referenced Documents (purchase separately) The documents listed below are referenced within the subject standard but are not provided as part of the standard.
Tag and Label Manufacturers Institute, Inc. (TLMI) StandardL-IB1 TLMI Loop Tack Test
A666 Specification for Annealed or Cold-Worked Austenitic Stainless Steel Sheet, Strip, Plate, and Flat Bar
D907 Terminology of Adhesives
D2651 Guide for Preparation of Metal Surfaces for Adhesive Bonding
E4 Practices for Force Verification of Testing Machines
E171 Practice for Conditioning and Testing Flexible Barrier Packaging
E177 Practice for Use of the Terms Precision and Bias in ASTM Test Methods
E691 Practice for Conducting an Interlaboratory Study to Determine the Precision of a Test Method
European Association for the Pre-Adhesed Labeling Industry (FINAT) StandardFTM 9
ICS Number Code 83.180 (Adhesives)
UNSPSC Code 31201626(Pressure sensitive adhesive PSA)
|Link to Active (This link will always route to the current Active version of the standard.)|
ASTM D6195-03(2019), Standard Test Methods for Loop Tack, ASTM International, West Conshohocken, PA, 2019, www.astm.orgBack to Top